over the past years , the design and synthesis of nanostructured materials with desired size , shape , and morphology have attracted considerable attention for achieving novel morphology - dependent chemical  physical properties.[1 - 8 ] particularly , porous nanostructure materials have received significant interest owing to the pore structure features and the large specific surface area , which make them suitable for applications in catalysis , sensing , energy storage , etc.[9 - 16 ] glucose monitoring is vital in clinical diagnostics , biotechnology , and the food industry .
specifically , there has been great interest in the development of electrochemical glucose sensors . compared with other detection approaches ,
the use of an electrochemical technique is one of the most promising in the construction of simple and low - cost glucose sensors because of its high sensitivity , good selectivity , and ease of operation .
the conventional glucose biosensors based on glucose oxidase ( god ) exhibit high sensitivity and selectivity .
however , due to the intrinsic features of enzymes , these god - based biosensor approaches suffer greatly from the influences of various environmental factors such as temperature , humidity , ph value , organic reagents , and toxic chemicals.[18 - 21 ] to solve these problems , nonenzymatic glucose biosensors based on the direct detection of glucose have been developed for practical applications .
recent research has shown that nanomaterials can be applied as sensors for glucose detection because of their unique physical and chemical properties .
for example , noble metals , metal alloys , and metal oxides have been successfully used in the construction of nonenzymatic glucose sensors,[22 - 28 ] suggesting that nanostructured materials are potential candidates for application as nonenzymatic glucose sensors . as an important ii  vi semiconductor material ,
zns has been extensively studied due to its luminescent , photochemical , and electrochemical properties .
,   nis has also been widely studied and has widespread applications in lithium ion batteries , supercapacitors , waste water treatment , etc.[31 - 33 ] the individual physical and chemical properties of zns or nis materials have been extensively studied ; however , there have been few reports on zns 
recently , much attention has been focused on improving the related physical and chemical performance of materials based on mixed transition metal sulfides , which can provide a synergistic effect of all individual constituents and efficient rapid pathways for ion and electron transport not only at the surface of materials , but also throughout the bulk of materials.[34 - 36 ] although many simple metal sulfides have been prepared , the controllable preparation of mixed transition metal sulfides with desirable composition and morphology still remains a great challenge .
thus , developing simple routes to prepare mixed transition metal sulfides is necessary . in this work
nis composite has two advantages : 1 )  it provides a large enough inner space and a high active surface area due to a strong synergistic effect from zns and nis ; 2 )  as electrochemical active materials for nonenzymatic glucose sensors , the synthesized zns 
moreover , the sensor is also highly selective to the target analyte . the mesoporous zns 
nis mesoporous materials was performed via a simple ion - exchange reaction between ni and zns nanospheres .
figure  1 presents the x - ray diffraction ( xrd ) patterns of the prepared samples .
all the diffraction peaks can be perfectly indexed to the pure hexagonal phase of zns with lattice parameters a=0.3821  nm and c=0.6257  nm , which are in good agreement with the international center for diffraction datas joint committee on powder diffraction standards ( jcpds ) card 36 - 1450 .
the xrd pattern shows that the diffraction peaks of ( 100 ) and ( 101 ) overlap with the diffraction peak of ( 002 ) because of widening , which is a result of the small crystallite size .
no characteristic peaks corresponding to other impurities were observed in the pattern , which indicates that the products are pure zns ( figure  1  a ) .
figure  1  b shows the xrd pattern of the prepared zns  nis composites .
x - ray diffraction ( xrd ) patterns of a )  zns and b )  zns  nis composite materials . to gain further information on the elemental compositions of the zns  nis composites , x - ray photoelectron spectroscopy ( xps ) was used to further characterize the sample .
the two strong peaks at 1020.8 and 1044.1  ev , assigned to the binding energies of zn 2p3/2 and zn 2p1/2 , respectively , suggest the existence of zn . the ni 2p xps spectrum is shown in figure  2  c ; two major peaks with binding energies at 855.3 and 872.8  ev
in addition , a weak peak corresponding to the satellite peak at around 861.2  ev was also observed , which was ascribed to the multi - electron excitation ( shake - up signal ) .
high - resolution scans of the s element in figure  2  d reveal a peak centered at around 160.6  ev , which can be accordingly assigned to the binding energy of s 2p .
the corresponding energy dispersive x - ray spectroscopy ( eds ) maps of the zns 
nis composites were also recorded ( figure  s1 , supporting information ) to further confirm the zn , ni , and s elements . in figure  s1
three color mapping images are shown : red : znk , green : nik , and blue : sk .
for the different element contents , the green nik color is much lighter than the red znk images , which reveals that the ni content is much lower than the zn content .
it was found that the ni element content is about 4.5  at  % .
high resolution x - ray photoelectron spectroscopy ( xps ) survey scan spectra of the zns  nis composites : a )  full survey scan ; b )  zn  2p ; c )  ni  2p ; d )  s  2p
. the morphology of zns and zns  nis composites were investigated by electron microscopy .
typical scanning electron microscopy ( sem ) and transmission electron microscopy ( tem ) images are shown in figure  3  a  d .
the prepared zns particles are monodisperse solid spheres with average diameters of 500  nm , and the surfaces of these spheres are relatively rough ( figure  3  a , b ) , suggesting that the zns solid nanospheres contain a large number of packed nanoparticles , which is further confirmed by the corresponding highly enlarged tem image ( see inset in figure  3  d ) .
a high - resolution tem image ( figure  3  e ) displays several sets of lattice fringes with a spacing of 0.33  nm , corresponding to the ( 100 ) planes of hexagonal phase zns crystals .
the selected area electron diffraction ( saed ) patterns confirm that the obtained zns are polycrystalline .
nis composites were also examined using tem . the tem image in figure  4  a shows zns 
nis composite nanospheres becomes rougher ( figure  4  b ) , suggesting the formation of nis crystallites on the zns surface .
nis composites in figure  4  d displays the lattice planes of zns ( 100 ) and nis ( 110 ) with lattice spacings of 0.33 and 0.17  nm , respectively .
scanning electron microscopy ( sem ) images of zns ( a , b ) ; transmission electron microscopy ( tem ) images of zns ( c , d ) , inset : highly enlarged section of the image ; e )  high - resolution tem image of the zns shell ; f )  selected area electron diffraction ( saed ) patterns of zns .
nis composites ( a  c ) ; d )  high - resolution tem image of the area marked with a white circle in panel  c. the specific surface areas and pore size of the prepared zns and zns  nis composites were further studied by nitrogen adsorption  desorption measurements , as indicated in figure  5 .
the hysteresis loop of the zns and zns  nis composites typically belongs to type  iv , indicating the characteristics of a mesoporous material . as shown in figure  5  a , the specific surface area of zns 
nis composites ( 137.9  m  g ) is much larger than that of zns ( 68.9  m  g ) .
halenda ( bjh ) pore size distribution curves ( figure  5  b ) show that the zns and zns  nis composites present a monomodal pore distribution , and the average pore diameter is about 2.4  nm . as widely reported , a large effective surface area usually offers many nanochannels for contacting the electrolyte through surface  interface interactions of nanoporous micro-/nano - structures .
desorption isotherms of the prepared samples ; b )  corresponding pore volume distribution ( dv dr ) against pore diameter curves of the prepared samples . to evaluate the electrochemical property of the prepared mesoporous zns 
nis composites , we carried out the cyclic voltammetry ( cv ) to investigate glucose oxidation and reduction .
nis composites using a modified glassy carbon ( gc ) electrode and a bare gc electrode in the absence and presence of 5  mm glucose in 0.1  m naoh .
as shown for the bare gc electrode , there is only a small background current observed ( figure  6  a ) , whereas a big increase in signal can be noted when the electrode was modified by the prepared mesoporous zns 
nis composites ( figure  6  b ) . upon the addition of 5  mm glucose
, a more dramatic increase can be found after the gc electrode was modified ( figure  6  c ) .
cyclic voltammetry ( cv ) traces : a )  bare gc electrode in glucose ( 5  mm ) and naoh ( 0.1  m ) ; gc electrode modified with zns  nis composites in naoh ( 0.1  m ) in the b )  absence or c )  presence of glucose ( 5  mm ) ; scan rate=50  mv  s. we also carried out cv to investigate glucose oxidation and reduction in physiological ph values ( ph  7.2 ) .
after the addition of 5  mm glucose , a small increase of signal can be noted ( figure  s2 , supporting information ) .
nis composites have an excellent electroanalytical ability in 0.1  m naoh solution compared with solutions at physiological ph and an enhanced response that can be attributed to many transport channels in the mesoporous zns  nis composites materials owing to its high specific surface areas .
time responses at a potential of 0.6  v after successive injections of different amounts of glucose into the 0.1  m naoh solution under stirring are presented in figure  7  a. it can be seen from the insets of figure  7  a that a gc electrode modified with mesoporous zns 
nis composites shows an obvious increase in current response after successive additions of glucose , and it takes less than 5  s to achieve the steady - state current upon addition of glucose to the stirring support electrolyte .
nis composites could be attributed to the synergistic effect of the composites , which include highly active catalytic sites for glucose oxidation owing to the high specific surface areas .
the high electron - transfer rate can be associated with the many transport channels throughout the mesoporous zns  nis composite materials . in figure  7  b
, we find the glucose detection concentration range to be 0.125  m0.12  mm ( r=0.9968 ) , and the calculated sensitivity is 48.5  a  mm . in the glucose concentration range of 0.15  mm1.0  mm ( r=0.9935 ) ,
the calculated sensitivity is 26.4  a  mm . the performance of the prepared mesoporous zns 
nis composites is comparable with some nonenzymatic glucose sensors , as shown in table  s1 ( supporting information ) . the sensitivity and detection limit of glucose for the mesoporous zns  nis composite electrocatalyst are better than those of many nonenzymatic sensors , such as ptni nanoparticles / graphene ( 20.42  a  mm  cm , 0.01  mm ) , palladium nanotube ( 33.19  a  mm , 0.1  mm ) , and nio / dna - dispersed graphene hybrid ( 9  a  mm  cm , 2.5  m ) . ,   however , the sensitivity and detection limit of some nonenzymatic sensors are better than our results , such as for porous ni networks ( 2900  a  mm  cm , 0.07  m ) and cuo  nio microfibers ( 3165.53  a  mm  cm , 1  nm ) .
a )  current  time response diagram of a gc electrode modified with mesoporous zns 
nis composites upon successive addition of glucose in naoh ( 0.1  m ) ( inset : magnified diagram at glucose concentrations of 0.1255  m ) ; b )  plot of electrocatalytic current of glucose versus its concentrations in the range of 0.125  m1.0  mm ; c )  amperometric response of modified electrodes with successive addition of glucose , ascorbic acid ( aa ) , uric acid ( ua ) , dopamine ( da ) , kcl , and glucose in naoh ( 0.1  m ) .
one of the major challenges in nonenzymatic glucose detection is to eliminate the electrochemical response generated by some easily oxidizable endogenous interfering compounds such as ascorbic acid ( aa ) , uric acid ( ua ) , dopamine ( da ) , and kcl . owing to their higher electron transfer rates
nis composite electrode with highly active surfaces can favor a kinetically controlled sluggish reaction ( the oxidation of glucose ) to a greater extent than diffusion - controlled reactions ( the oxidation of interfering species ) .
therefore , interference tests were carried out by adding 100  m glucose , followed with additions of 200  m aa , 200  m ua , 200  m da , and 200  m kcl in 0.1  m naoh .
the results shown in figure  7  c demonstrate that almost negligible interference from aa , ua , da , and kcl is present at the sensor .
nis composites exhibit high selectivity , which is might attributed to the morphological characteristics of a mesoporous structure with high specific surface area and a rational composition of the two constituents .
nis composites on the surface of electrodes can be used to modify the mass transport regime , and under favorable circumstances , this alteration can facilitate the amperometric discrimination between species.[45 - 47 ] thus , zns  nis sensors exhibit high selectivity .
nis mesoporous materials were made , and their current responses to 10  m glucose were investigated .
the relative standard deviation ( rsd ) was 3.51  % with a mean current response of 0.0739  a .
nis / gc electrodes response current over 4000  s after the addition of 10  m glucose . after 4000  s
, there is only a 6  % loss in the specific response current of the electrode , which is stable enough for use as an electrochemical sensor of glucose .
nis composites after the addition of glucose ( 10  m ) measured over 4000  s. based on the discussion above , the prepared mesoporous zns 
nis composites can offer a larger accessible surface area for the nanopores , a short diffusion path for ions , and good conductivity .
nis composites could have novel interfaces ( between the zns and nis nanoparticles ) , which can provide a synergistic effect from individual constituents and efficient , rapid pathways for ion and electron transport not only at the materials surface , but also throughout the bulk of the material .
physical adsorption  desorption abilities towards ions and their diffusion paths , resulting in a better electroanalytical detection of glucose.[48 - 50 ]
nis composites have been prepared by ion - exchange reactions using zns as a precursor . as a result of novel interface characteristics , conductivity , and synergistic effects from zns and nis constituents , the mesoporous zns 
nis composites provide an efficient and rapid pathway for ion and electron transport not only at the materials surface , but also throughout the bulk of the material .
the results of the electrochemical detection show the mesoporous zns  nis composites exhibit high selectivity and a low detection limit for the oxidation of glucose .
this present study is important as it provides us with an effective approach in preparing novel mesoporous zns 
this synthesis method can be extended to the preparation of other materials for many applications .
materials preparation : zns nanospheres were prepared as follows : zn(ac)26  h2o ( 0.5  mmol ) was dissolved in glycerol ( 8.0  ml ) and h2o ( 9.0  ml ) with magnetic stirring , then nh3 solution ( 3.0  ml , 25  % , analytically pure ) and l - cysteine ( 3.0  mmol ) were added , respectively . after 10  min of stirring at rt , the mixture was transferred into a 50  ml teflon - lined autoclave reactor and heated in an oven at 140  c for 6  h. the precipitate was centrifuged ( 4000  rpm for 10  min ) and washed with deionized h2o ( 10  ml ) and absolute ethanol ( 10  ml ) , and dried in a vacuum oven at 50  c for 12  h. to prepare zns 
nis mesoporous composites , zns ( 1.0  mmol ) nanospheres were dispersed in deionized h2o ( 20  ml ) .
then , ni(ac)24  h2o ( 248.8  mg , 1.0  mmol ) was added to the solution while stirring .
the resulting mixture was then transferred into a 100  ml round - bottom flask and heated at 80  c for 24  h using a water bath .
the precipitate was collected by centrifugation ( 4000  rpm for 10  min ) and washed with deionized h2o ( 10  ml ) and absolute ethanol ( 10 ml ) , then dried at 50  c for 12  h. preparation of the glucose sensor : the glassy carbon ( gc ) electrode ( 3  mm diameter ) was carefully polished using a polishing cloth with alumina slurry ( 1.0 , 0.3 , and 0.05  m in sequence ) , then rinsed thoroughly with deionized h2o , and allowed to dry at rt . to prepare the gc electrode modified with the zns 
nis composite ( 1  mg  ml ) was prepared , and the suspension ( 5  l ) was cast onto the surface of the pretreated gc electrode . the solvent was allowed to evaporate at rt , leaving the zns  nis mesoporous material immobilized on the gc electrode surface . apparatus and measurements : cyclic voltammetry ( cv ) measurements were performed on a chi 660d electrochemical station ( chen hua , shanghai , china ) , a three - compartment electrochemical cell containing a saturated calomel reference electrode , a platinum wire auxiliary electrode , and a modified gc electrode as the working electrode .
for the cv measurements , the potential scan was taken from 0.60 to 1.00  v at a scan rate of 50  mv  s. for the amperometric detection , all measurements were performed by applying an appropriate potential to the working electrode and allowing the transient background current to decay to a steady - state value prior to the addition of glucose .
characterization : the morphology of the obtained sample was observed by a hitachi s-4800 field emission scanning electron microscope ( fe - sem ) at an acceleration voltage of 10.0  kv .
the phase analyses of the samples were characterized by x - ray diffraction ( xrd ) on a shimadzu xrd-6000 powder x - ray diffractometer with cu- radiation ( =1.5418   ) .
standard and high - resolution ( hr ) transmission electron microscopy ( tem ) images were obtained on a jeol jem-2100 microscope at an acceleration voltage of 200  kv .
the surface area , pore size , and pore size distribution of the materials were determined by brunauer 
 desorption and barett  joyner  halenda ( bjh ) methods on a micromimetrics asap2020 physisorption analyzer .
as a service to our authors and readers , this journal provides supporting information supplied by the authors .
such materials are peer reviewed and may be re - organized for online delivery , but are not copy - edited or typeset . technical support issues arising from supporting information ( other than missing files ) should be addressed to the authors .
 mesoporous zns  
 nis composites are prepared via ion- exchange reactions using zns as the precursor . the prepared mesoporous zns  
 nis composite materials have large surface areas ( 137.9  m2  g1 ) compared with the zns precursor . 
 more importantly , the application of these mesoporous zns  nis composites as nonenzymatic glucose sensors was successfully explored . 
 electrochemical sensors based on mesoporous zns  nis composites exhibit a high selectivity and a low detection limit ( 0.125  m ) toward the oxidation of glucose , which can mainly be attributed to the morphological characteristics of the mesoporous structure with high specific surface area and a rational composition of the two constituents . in addition , the mesoporous zns  
 nis composites coated on the surface of electrodes can be used to modify the mass transport regime , and this alteration can , in favorable circumstances , facilitate the amperometric discrimination between species . 
 these results suggest that such mesoporous zns  
 nis composites are promising materials for nonenzymatic glucose sensors . 
Introduction
Results and Discussion
Conclusions
Experimental Section
Supporting Information